View metadata, citation and similar papers at core.ac.uk brought to you by CORE

provided by Springer - Publisher Connector

Article

Condensed Matter Physics March 2012 Vol.57 No.7: 719723 doi: 10.1007/s11434-011-4945-6

Density and structure of undercooled liquid titanium

WANG HaiPeng, YANG ShangJing & WEI BingBo*

Department of Applied Physics, Northwestern Polytechnical University, Xi’an 710072, China

Received October 29, 2011; accepted December 16, 2011

For liquid Ti, it is difficult to achieve high undercooling because of its chemical reactivity; as a result, there is little information available on its properties and structure in the undercooled state. In this study, we investigate the density and structure, using mo- lecular dynamics method, for the undercooling and superheating ranges 0–743 K and 0–457 K. The density increases quadratically for undercooling. At the melting temperature, the density is 4.14 g/cm3, and first and second temperature coefficients are obtained. The pair correlation functions and coordination numbers indicate that the short range degree of order becomes increasingly sig- nificant with increasing undercooling.

liquid metal, undercooling, density, liquid structure, titanium

Citation: Wang H P, Yang S J, Wei B B. Density and structure of undercooled liquid titanium. Chin Sci Bull, 2012, 57: 719723, doi: 10.1007/s11434-011-4945-6

In comparison with the majority of normal-state liquids, densities of liquid Ti. Rhim et al. [7] measured the density undercooled liquid metals display many unusual character- of liquid Ti in the temperature range 1650–2000 K using an istics as a result of their thermodynamic metastability. This electrostatic levitator (ESL). Paradis et al. [8] obtained the is particularly seen for metals with high melting-tempera- density of liquid Ti using an ESL method in the temperature tures and these have attracted increasing research interest in range 1750–2050 K. Ishikawa et al. [9] also reported the the past ten years [1–6]. The densities and structures of density obtained using their ESL facility in the temperature metastable undercooled liquids are of great importance in range 1680–2060 K. However, there are some discrepancies understanding metastable liquid metals. However, little is among these reported results. Detailed investigations of the known about the densities and structures of metastable liq- densities are still needed and the temperature regimes stud- uid metals compared with those of stable liquids above the ied so far have not been broad enough. In order to further melting temperatures. understand the physical characteristics of liquid Ti, density Ti is widely used in various applications such as air- changes and liquid structures are required over a broad frames and turbine blades because it has excellent properties, temperature range, especially for the metastable under- including excellent strength, low density, good ductility, cooled regime. and superior resistance to chemical processes. However, its The liquid structure is also of importance in studies of melting temperature is very high, at 1943 K, which is espe- undercooled liquid Ti. However, it is extremely difficult to cially for high reactivity in the liquid state. These factors obtain detailed structural information because of its meta- cause great difficulties in the experimental determination of stable characteristics and rapid atom diffusion. Recently, an the properties of liquid Ti. Accordingly, information on the experimental investigation of the liquid structures of metals density and liquid structure is scarce. The requirement for was performed by combining containerless processing with this information is increasing as a result of the extensive X-ray scattering, synchrotron X-ray diffraction, and neutron application of Ti in various industrial alloys. diffraction methods [10–13]. For liquid Ti, Lee et al. [14] In the past ten years, several researchers have reported measured the structure factor of an electrostatically levitated Ti droplet at 282 K undercooling by synchrotron X-ray dif- *Corresponding author (email: [email protected]) fraction, and Holland-Moritz et al. [15] determined the

© The Author(s) 2012. This article is published with open access at Springerlink.com csb.scichina.com www.springer.com/scp 720 Wang H P, et al. Chin Sci Bull March (2012) Vol.57 No.7 structure factor of liquid Ti at about 200 K undercooling by and materials design. The density of liquid Ti is calculated neutron scattering combined with an electromagnetic levita- as a function of temperature, as illustrated in Figure 1. The tion technique. However, many problems with respect to the density exhibits a nonlinear dependence on the tempera- density and structure of liquid Ti still need to be resolved. ture T: Molecular dynamics method, combining with a reasona- 4.14 2.15 1048 (TT ) 3.71 10 ( TT )2(g/cm3), (2) ble potential model, has been used to simulate the properties mm and liquid structures of undercooled metals [16–19]. Com- where the melting point Tm is equal to 1943 K. The calcu- pared with experimental studies, high undercooling is easily lated temperature for the density of liquid Ti is in the range achieved in simulations, and more detailed information can 1200–2400 K, including 743 K undercooling and 457 K therefore be accordingly obtained. The objective of the pre- superheating. Such a large undercooling is hard to achieve sent work is to study the density and structure of metastable experimentally. From eq. (2), the density at the melting undercooled Ti over a much broader temperature range than temperature is 4.14 g/cm3, and its first and second tempera- those previously studied. Subsequently, the molar volume 4 3 1 8 ture coefficients are 2.1510 g cm K and 3.7110 and thermal expansion coefficient are also derived. g cm3 K2. Figure 1 also presents the density results for liquid Ti 1 Materials and method obtained by other researchers, for evaluation of the present results obtained by molecular dynamics methods. Rhim et al. [7] measured the density of liquid Ti in the temperature Selection of the potential model is very important for the range 1650–2000 K using an ESL, and the following linear final calculated results. In density functional theory, the expression was obtained: modified embedded atom method (MEAM) was proposed 4 3 by Baskes, based on the potential model of an embedded 4.208 5.08 10 (TTm ) (g/cm ). (3) atom method [20]. As well as describing metals with cubic structure, the MEAM model can also deal with metals with This result is also illustrated in Figure 1, and includes a hexagonal structures, including Ti [21,22]. The MEAM maximum undercooling of 293 K, as marked by line 1. It potential model is expressed by [20] can be seen that Rhim’s result is larger than the present result. At the melting temperature, only a difference of 0.07 g/cm3 1 exists between the two results, i.e. Rhim’s result of 4.208 E Fr() (), (1) 3 3 tot i i ij ij g/cm is 1.6% larger than the present value of 4.14 g/cm . ii2 ,(ji j ) However, the present temperature coefficient is larger than where Fi is the energy of the embedded atom i in an electron that obtained by Rhim’s experiments. density i, i,j is a pair of potential interactions between at- Paradis et al. [8] measured the density of liquid Ti using oms i and j, which is summed over all neighbors j of atom i an ESL method and derived the following correlation: within the cutoff distance. 4.10 9.90 104 (TT ) (g/cm3), (4) In the present work, 32000 Ti atoms are arranged in a m cubic box as the liquid structure. The system is subjected to where the experimental temperature range is 1750–2050 K, periodic boundary conditions in three dimensions under and includes a maximum undercooling of 193 K. The present constant pressure and constant temperature. The time step is calculated value of the density at the melting temperature is 1 fs and the pressure is set to 105 Pa. The temperature is adjusted every 50 steps. It starts at 3000 K to obtain an equilibrium liquid state. The initial temperature is kept con- stant for 200000 steps. The cooling process, with a cooling rate of 1013 K/s, is performed for calculations at 100 K temperature intervals. At each temperature, 100000 steps are carried out for equilibrium. The last 50000 steps are used to calculate the final results. During the calculations, the system is kept in a liquid state by monitoring the pair-distribution function (PDF) and the mean-square dis- placement versus the simulated time. All codes are run in a Lenovo 1800 Cluster system.

2 Results and discussion

Density data play a fundamental role in numerical modeling Figure 1 Density of liquid Ti versus temperature. Wang H P, et al. Chin Sci Bull March (2012) Vol.57 No.7 721 very close to Paradis’s experimental result. However, there is a large difference between the two temperature coefficients. Ishikawa et al. [9] also determined the density of liquid Ti using their ESL facility and derived the following rela- tionship:

4 3 4.17 2.2 10 (TT m ) (g/cm ), (5) where the experimental temperature range is 1680–2060 K, and includes a maximum undercooling of 263 K. The density of liquid Ti in Smithells Metals Reference Book [23] is

4 3 4.13 2.3 10 (TT m ) (g/cm ). (6) Figure 2 Molar volume and thermal expansion coefficient of liquid Ti According to the above analysis, the maximum under- versus temperature. coolings achieved by Rhim, Paradis, and Ishikawa are 293, 193 and 263 K, respectively. In Smithells Metals Reference than that at the melting point. For solid Ti, Vm is 10.64 Book [23], only the data for the density of liquid Ti above 3 the melting temperature are given. The four previously ob- cm /mol at room temperature. This means that the value Vm tained densities at the melting temperature are as follows: for liquid Ti at 1943 K is 8.6% larger than that of solid Ti at Rhim’s result is 4.208 g/cm3, Paradis’s result is 4.10 g/cm3, 293 K. For the maximum undercooling of 768 K, the molar Ishikawa’s result is 4.17 g/cm3, and the result in [13] is 4.13 volume of liquid Ti is 5.2% larger than that of solid Ti at g/cm3. The present value is 4.14 g/cm3. Among these results, room temperature. This indicates that the structure of liquid the maximum is Rhim’s value of 4.208 g/cm3, the minimum Ti may change accordingly. value is Paradis’s result of 4.10 g/cm3, and the difference The thermal expansion coefficient β can be expressed as 3 between them is 0.108 g/cm . Such a small difference is 1 . (8) quite satisfactory. T However, there are large differences among the temper- ature coefficients reported by different researchers. Para- Based on the above equations and the density results, the dis’s temperature coefficient, 9.9104 g cm3 K1, is the thermal expansion coefficients of liquid Ti are computed minimum. The second lowest, 5.08104 g cm3 K1, is and shown in Figure 2; they can be expressed as Rhim’s result, and the others are approximate. Although 4.88 4.64 1058TT 5.74 102 . (9) there are no significant differences among the density val- ues at the melting temperature, the deviations among these The thermal expansion coefficient increases nonlinearly results become increasingly large when the temperature with increasing temperature coefficient. The thermal expan- deviates from the melting temperature for either the super- sion coefficients of liquid Ti are of the order of magnitude heated state or the undercooled state. In terms of the above 105. However, those of solid Ti are of the order of magni- analysis, the present results agree well with Ishikawa’s re- tude 106; for example, at 373 K is 8.8106 K1, and at sults (line 3) and the data in [13] (line 4). Accordingly, it 1073 K is 9.9106 K1. It can be seen that for Ti in the can be concluded that our molecular dynamics simulation liquid state is much larger than that of solid; this may be provides reasonable density data for liquid Ti, especially for because the inter-atomic forces in liquid metals are much a highly undercooled state. weaker than those in solid metals. According to the present density, important physical Furthermore, the liquid structure of Ti can be represented properties such as the molar volume and thermal expansion by the PDF; this is computed using the equation g(r)=V

Figure 2 shows that Vm increases nonlinearly with in- undercooling is sufficiently large to enable the study of 3 creasing temperature; Vm is 11.56 cm /mol at the melting structural changes at the atomic scale. For clarity, only the 3 temperature of 1943 K, but Vm drops to 11.19 cm /mol PDFs at four temperatures, 2400 K (highly superheated when the undercooling achieves 743 K. It is evident that the state), 2000 K (near the melting temperature), 1600 K (un- molar volume at the maximum undercooling is 3.3% smaller dercooled state), and 1200 K (highly undercooled state) are 722 Wang H P, et al. Chin Sci Bull March (2012) Vol.57 No.7 presented in Figure 3. In Figure 3, clear peaks exist at the first-neighbor dis- tance. With increasing distance, the PDF values approxi- mate to 1. This suggests that the Ti atoms in the simulated system are ordered in the short range and disordered in the long range. These are typical characteristics of liquids. Alt- hough the four PDFs look similar to each other, there are still some differences among them. The first peak heights of the PDFs change significantly with temperature; this repre- sents the degree of order of the Ti atoms at the first-neighbor distance. For the peaks at the sub-neighbor distance, a sad- dle occurs at 2400 K, the saddle changes to two small peaks at 2000 K, to two obvious peaks instead of a saddle at 1600 K, and three small peaks appear at 1200 K, indicating that the liquid structure of Ti changes when liquid Ti changes from a highly superheated state to a metastable undercooled state. Figure 4 illustrates the PDF heights at the first- and sub- neighbor distances of liquid Ti. The PDF values at R1 (Fig- ure 4(a)) decrease with increasing temperature. At 1200 K, the PDF at R is 4.95, which is 43% larger than the value of 1 Figure 4 Pair distribution function heights at (a) first- and (b) sub- 3.47 at 2400 K. It is apparent that the degree of order of the neighbor distances of liquid Ti versus temperature. atom distribution increases from the normal liquid to the undercooled liquid. The second peaks are also analyzed at The coordination number of liquid Ti is also computed to different temperatures, and are shown in Figure 4(b). The analyze the liquid structure. First, the cutting distances r features are similar to those of the PDFs at R , and the PDFs c 1 are determined from the first PDF peaks, as shown in Figure at R increase with increased undercooling. Comparing the 2 5. It can be seen that r slightly increases with increasing PDF at R at 1200 K with that at 2400 K shows that the c 2 temperature. The coordination number is almost independ- value is enhanced by 32% when liquid Ti cools from a su- ent of the temperature, and is in the range 10.0–10.3 from perheated state at 2400 K to a highly undercooled state at 1200 to 2400 K. This is different from the characteristics of 1200 K. the PDF peak heights.

3 Concluding remarks

In summary, the densities and structures of liquid Ti were investigated in the temperature range 1200–2400 K, includ- ing both superheated and undercooled states. The density

Figure 5 Coordination number and cutting distance of liquid Ti versus Figure 3 Pair distribution functions of liquid Ti versus temperature. temperature. Wang H P, et al. Chin Sci Bull March (2012) Vol.57 No.7 723 increases nonlinearly with increased undercooling. At the Bi-Ga hypermonotectic alloy under acoustic levitation condition. melting temperature, the density is 4.14 g/cm3, and its first and Chin Sci Bull, 2007, 52: 1446–1450 4 3 1 6 Wang H P, Chang J, Wei B. Measurement and calculation of surface second temperature coefficients are 2.1510 g cm K tension for undercooled liquid nickel and its alloy. J Appl Phys, 2009, and 3.71108 g cm3 K2. The present work provides den- 106: 033506 sity values over a broader temperature range, especially for 7 Paradis P F, Rhim W K. Non-contact measurements of thermophysi- cal properties of titanium at high temperature. J Chem Thermodyn, larger undercooling regimes, than those in previous studies. 2000, 32: 123–133 The maximum undercooling is 743 K. Such a large under- 8 Paradis P F, Ishikawa T, Yoda S. Experiments in materials science on cooling is hard to achieve experimentally. Based on the the ground and in reduced gravity using electrostatic levitators. Adv highly accurate calculated density, the molar volume and Space Res, 2008, 41: 2118–2125 9 Ishikawa T, Paradis P F. Thermophysical properties of molten re- thermal expansion coefficient are derived; these increase fractory metals measured by an electrostatic levitator. J Electron Mater, quadratically with increasing temperature. 2005, 34: 1526–1532 The PDF heights at the first-neighbor distance increase 10 Kordel T, Holland-Moritz D, Yang F, et al. Neutron scattering ex- periments on liquid droplets using electrostatic levitation. Phys Rev B, with decreasing temperature. For 1200 K, the PDF at R1 is 2011, 83: 104205 4.95, which is 43% larger than the value of 3.47 at 2400 K. 11 Kalay I, Kramer M J, Napolitano R E. High-accuracy X-ray diffrac- The PDF at the sub-neighbor distance is similar to the PDF tion analysis of phase evolution sequence during devitrification of at R1, which increases with increased undercooling. A com- Cu50Zr50 metallic glass. Metall Mater Trans A, 2011, 42A: 1144–1153 parison of the PDF at R2 at 1200 K with that at 2400 K 12 Higuchi K, Kimura K, Mizuno A, et al. Density and structure of un- shows that the value is enhanced by 32% when liquid Ti dercooled molten silicon using synchrotron radiation combined with cools from a superheated state at 2400 K to a highly under- an electromagnetic levitation technique. J Non-Cryst Solids, 2007, cooled state at 1200 K. The above characteristics indicate 353: 2997–2999 that the degree of order of the atom distribution increases 13 Kim T H, Lee G W, Sieve B, et al. In situ high-energy X-ray diffrac- tion study of the local structure of supercooled liquid Si. Phys Rev from the normal liquid to the undercooled liquid. However, Lett, 2005, 95: 085501 the coordination number changes little, and remains in the 14 Lee G W, Gangopadhyay A K, Kelton K F, et al. Difference in ico- range 10.0–10.3 from 1200 K to 2400 K. sahedral short-range order in early and late transition metal liquids. Phys Rev Lett, 2004, 93: 037802 15 Holland-Moritz D, Heinen O, Bellissent R, et al. Short-range order of This work was supported by the National Natural Science Foundation of stable and undercooled liquid titanium. Mater Sci Eng A, 2007, 449: China (50971103 and 50971105), the Program for New Century Excellent 42–45 Talents, the Natural Science Foundation of Shaanxi Province (2010JQ6004), 16 Jakse N, Pasturel A. Dynamics of liquid and undercooled silicon: An the Shaanxi Project for Young New Star in Science and Technology and the ab initio molecular dynamics study. Phys Rev B, 2009, 79: 144206 NPU Foundation for Fundamental Research. 17 Gheribi A E. Molecular dynamics study of stable and undercooled liquid zirconium based on MEAM interatomic potential. Mater Chem Phys, 2009, 116: 489–496 1 Shen Y T, Kim T H, Gangopadhyay A K, et al. Icosahedral order, 18 Morishita T. How does tetrahedral structure grow in liquid silicon frustration, and the glass transition: Evidence from time-dependent upon supercooling. Phys Rev Lett, 2006, 97: 165502 nucleation and supercooled liquid structure studies. Phys Rev Lett, 19 Wang H P, Chang J, Wei B. Density and related thermophysical 2009, 102: 057801 properties of metastable liquid Ni-Cu-Fe ternary alloys. Phys Lett A, 2 Pietropaolo A, Senesi R, Andreani C, et al. Excess of proton mean 2010, 374: 2489–2493 kinetic energy in supercooled water. Phys Rev Lett, 2008, 100: 20 Baskes M I. Modified embedded-atom potentials for cubic materials 127802 and impurities. Phys Rev B, 1992, 46: 2727–2742 3 Ganesh P, Widom M. Liquid-liquid transition in supercooled silicon 21 Zhang J M, Wang D D, Xu K W. Calculation of the surface energy of determined by first-principles simulation. Phys Rev Lett, 2009, 102: hcp metals by using the modified embedded atom method. Appl Surf 075701 Sci, 2006, 253: 2018–2024 4 Luo B C, Wang H P, Wei B. Phase field simulation of monotectic 22 Kim Y M, Lee B J, Baskes M I. Modified embedded-atom method transformation for liquid Ni-Cu-Pb alloys. Chin Sci Bull, 2009, 54: interatomic potentials for Ti and Zr. Phys Rev B, 2006, 74: 014101 183–188 23 Gale W F, Totemeier T C. Smithells’ Metals Reference Book. 8th ed. 5 Hong Z Y, Lu Y J, Xie W J, et al. The liquid phase separation of Burlington: Elsevier Butterworth Heinemann, 2004. 14-10

Open Access This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and source are credited.